Cite This: J. Am. Chem. Soc. 2019, 141, 11253−11258 pubs.acs.org/JACS
Multistep Solid-State Organic Synthesis of Carbamate-Linked Covalent Organic Frameworks † † ‡ † † ‡ Steven J. Lyle, Thomas M. Osborn Popp, , Peter J. Waller, Xiaokun Pei, Jeﬀrey A. Reimer, † § and Omar M. Yaghi*, , † Department of Chemistry, University of CaliforniaBerkeley, Materials Sciences Division, Lawrence Berkeley National Laboratory, Kavli Energy NanoSciences Institute at Berkeley and Berkeley Global Science Institute, Berkeley, California 94720, United States ‡ Department of Chemical and Biomolecular Engineering, Environmental Energy Technologies Division, Lawrence Berkeley National Laboratory, University of CaliforniaBerkeley, Berkeley, California 94720, United States § King Abdulaziz City for Science and Technology, Riyadh 11442, Saudi Arabia
*S Supporting Information
ABSTRACT: Herein, we demonstrate the ﬁrst example of a multistep solid-state organic synthesis, in which a new imine- linked two-dimensional covalent organic framework (COF- 170, 1) was transformed through three consecutive post- synthetic modiﬁcations into porous, crystalline cyclic carbamate and thiocarbamate-linked frameworks. These linkages are previously unreported and inaccessible through de novo synthesis. While not altering the overall connectivity of the framework, these chemical transformations induce signiﬁcant conformational and structural changes at each step, highlighting the key importance of noncovalent interactions and conformational ﬂexibility to COF crystallinity and porosity. These transformations were assessed using 15N multiCP-MAS NMR spectroscopy, providing the ﬁrst quantitation of yields in COF postsynthetic modiﬁcation reactions, as well as of amine defect sites in imine-linked COFs. This multistep COF linkage postsynthetic modiﬁcation represents a signiﬁcant step toward bringing the precision of organic solution-phase synthesis to extended solid-state compounds.
■ INTRODUCTION by those linkages. This has been demonstrated for a number of Covalent organic frameworks (COFs) are a class of designed, imine-linked COFs, the linkages of which were converted to secondary amides, secondary amines, thiazoles, oxazoles, and porous, crystalline materials built from the covalent linkage of 8−12 ﬁ quinolines. However, amide- and oxazole-linked COFs geometrically prede ned building units into two- and three- 15,16 dimensional extended networks.1,2 The ability to control the have been formed directly from molecular building units, and in principle, each of these linkages could be made directly,
Downloaded via UNIV OF CALIFORNIA BERKELEY on August 8, 2019 at 21:21:52 (UTC). relative positioning of chemical functionalities in covalently by employing a one-pot strategy whereby COFs are formed See https://pubs.acs.org/sharingguidelines for options on how to legitimately share published articles. linked solids represents an extension of organic chemistry into 3,4 from a reversible imine condensation followed by a less the solid state. This extension includes not only the ability to 17−20 crystallize these ordered networks from molecular building reversible or irreversible second step in situ. blocks but also the ability to treat the extended solids as In organic synthesis, we are not limited to compounds molecules. It has been demonstrated in numerous cases that accessible in a single synthetic step. The translation of chemical transformations can take place on COFs much as multistep organic synthesis to the solid state, however, requires they do in solution due to the ability of reactants and extending not only the chemistry but also the rigor of − byproducts to diﬀuse through the pores of a COF.5 7 Notably, characterization found in small-molecule synthesis to solids. ﬁ postsynthetic modiﬁcations can be performed on COF linkages Herein, we describe the rst extension of both these features of − without alteration of topology.8 12 Linkage transformations, in organic chemistry to covalent solids, achieved by the multistep ﬁ particular, distinguish themselves from reactions performed on postsynthetic modi cation of a COF to generate porous, molecules appended to solid supports, such as solid-phase crystalline cyclic carbamate and thiocarbamate-linked frame- peptide synthesis, because the stability, reactivity, and structure works accessible only through multistep synthesis. Each of a COF is largely deﬁned by its linkages.13,14 reaction in this synthesis involves transformation of the Postsynthetic modiﬁcation allows access to new linkage functionalities without the need to develop reaction conditions Received: May 2, 2019 capable of directly generating an ordered network reticulated Published: June 21, 2019
© 2019 American Chemical Society 11253 DOI: 10.1021/jacs.9b04731 J. Am. Chem. Soc. 2019, 141, 11253−11258 Journal of the American Chemical Society Article
Scheme 1. Synthesis of Cyclic Carbamate and Thiocarbamate-Linked COFs by a Three-Step Solid-State Synthesis
Figure 1. (a) FT-IR spectra of COFs 1−5, labeled with diagnostic stretching frequencies reported for each linkage. (b) PXRD patterns of COFs 1− − 5, demonstrating the retention of crystallinity through all but amine-linked 3. (c) N2 adsorption isotherms performed at 77 K for COFs 1 5, displaying permanent porosity for all but amine linked 3. Solid and open circles designate adsorption and desorption points, respectively. Uptake is ﬁ 3 ° de ned as cm of N2 at 1 atm and 0 C per gram of sample. material’s linkage and as such occurs with concomitant ■ RESULTS AND DISCUSSION structural changes, but preservation of the underlying topology. A new kgm topology COF, COF-170 (1), was synthesized Furthermore, each compound was analyzed by 15N multiple solvothermally from the condensation of (E)-3,3′,5,5′-tetrakis- cross-polarization magic angle spinning nuclear magnetic (4-aminophenyl)stilbene (TAPS) and 3,5-dimethoxytereph- resonance spectroscopy (multiCP-MAS NMR), allowing for thalaldehyde (DMTP) in a 5:5:1 mixture of o-dichloroben- ° the ﬁrst quantitative evaluation of chemical transformations in zene, 1-butanol, and 6 M AcOH at 120 C for 3 days. COF- 170 served as the starting material for the synthesis of COFs. This work sets a new standard for the execution and isostructural cyclic carbamate- and thiocarbamate-linked COFs evaluation of multistep chemical transformations of solids and (Scheme 1). This synthesis began ﬁrst with demethylation of in doing so lays the groundwork for further exploration of 1’s methoxy groups, followed by reduction of the imine linkage solid-state organic synthesis. with sodium cyanoborohydride and acetic acid in THF.21 This
11254 DOI: 10.1021/jacs.9b04731 J. Am. Chem. Soc. 2019, 141, 11253−11258 Journal of the American Chemical Society Article amine-linked COF (3) was then treated with 1,1′-carbon- yldiimidazole (CDI) or 1,1′-thiocarbonyldiimidazole (TCDI) and N,N-dimethylaminopyridine (DMAP) in dichloromethane to yield cyclic carbamate- (4) and thiocarbamate- (5) linked COFs, respectively.22 Between each of these steps, and prior to characterization, the intermediate compounds were subjected to thorough solvent exchange and activation to prepare the material for the subsequent transformation. In order to provide rigorous data consistency, all characterization, including 15N multiCP-MAS NMR spectroscopy, was performed on the same 33% 15N-labeled samples. All relevant synthetic procedures can be found in sections 2−4 of the Supporting Information. The progress of these transformations was initially monitored by FT-IR spectroscopy (Figure 1a). Demethylation Figure 2. 15N multiCP-MAS NMR spectra of 33% 15N-labled COFs of 1’s methoxy groups was observed through the disappearance − − − 1 5, colored to highlight the composition of each sample. Spinning of its ether C O C symmetric and asymmetric stretches at side bands are indicated by asterisks. 1038 and 1288 cm−1, respectively.23 Upon reduction of the imine linkages of 2, we observed the disappearance of its imine Table 1. Linkage Composition of COFs 1−5, Determined −1 a CN stretch at 1614 cm and the emergence of an amine from Peak Fitting of 15N MultiCP-MAS NMR Spectra C−N stretch at 1516 cm−1.10 After cyclization to carbamates and thiocarbamates, characteristic CO and CS stretches were observed at 1719 and 1156 cm−1, respectively, and corroborated by comparison to molecular models (see SI, section S5).24 Although diagnostic, FT-IR spectroscopy alone does not constitute evidence of reaction completeness and in this context cannot provide quantitative information on the composition of the analyzed COFs. 15N solid-state NMR spectroscopy provides an alternative means to clearly track the conversion between linkages across the multiple steps of this synthetic process. While commonly employed in the character- ization of COF linkage transformations, traditional CP-MAS NMR does not provide quantitative integrations of resonances due to variable polarization rates between 1H and the target nucleus across diﬀerent chemical functionalities. Quantitative solid-state NMR spectra may be achieved by direct observation 15 of N; however, long T1 relaxation times combined with the low sensitivity of the nucleus can make these measurements impractical. MultiCP-MAS NMR spectroscopy provides a means to measure quantitative solid-state NMR spectra in solids with reasonable measurement times.25,26 To date, the multiCP method has only been applied to the measurement of 13C NMR spectra. In applying this method to 15N, we found it necessary to enrich the sample due to its low natural abundance. However, full enrichment was not necessary to obtain routine spectra. 15N multiCP-MAS NMR of 33% 15N-labeled substrates yielded quantitative insight into the postsynthetic modiﬁcation process (Figure 2). In the spectrum of each COF, the primary resonance observed corresponds to the major product of the preceding reaction step. As the resonances for each chemical site showed some degree of inhomogeneous broadening due to structural disorder, resonances corresponding to diﬀerent sites were ﬁt to Gaussian lineshapes, and their relative areas were aComposition ranges given for 4 and 5 reﬂect the fact that primary compared (see SI, section S6). Using this method, the amines and secondary amines with adjacent methoxy groups present composition of each COF along the synthetic pathway was in 3 may be forming O-methyl carbamate and thiocarbamate species analyzed (Table 1). In imine-linked COFs 1 and 2, residual which contribute to the observed carbamate and thiocarbamate primary amine sites were found to make up 6 and 8% of total resonances. 15N sites, respectively. The chemical shifts of the imine sites within these two materials are distinct enough to enable experiment. In contrast to the imine resonances, the chemical monitoring of the demethylation step, which occurred in 91% shifts of the methoxy-adjacent, hydroxy-adjacent, and primary yield. The reduction of imine species in 2 to make 3 was found amine linkages cannot be clearly resolved. Nonetheless, the to be complete within the detection limit of the NMR relative composition of secondary amine linkages can be
11255 DOI: 10.1021/jacs.9b04731 J. Am. Chem. Soc. 2019, 141, 11253−11258 Journal of the American Chemical Society Article inferred under the assumption that the amount of primary in 1, and only the orientation which yields intramolecular amine remains unchanged after the reduction. Treatment of 3 hydrogen bonding is present in 2. This suggests that upon with CDI and DMAP aﬀords a material 4 in which 86% of 15N demethylation the COF undergoes a structural rearrangement sites are carbamates, and the remainder are a mixture of amine to adopt its most stable conformation (Scheme 2). sites. Thiocarbamate-linked 5 shows a similar conversion of 86% thiocarbamate with 14% mixed amines remaining. The Scheme 2. Reorientation of Hydroxyl Groups in the Solid carbamate and thiocarbamate resonances in 4 and 5 are likely a State after Demethylation mixture of species, as only the secondary amine with an adjacent hydroxyl group can form cyclic carbamates or thiocarbamates. The primary amines and the secondary amines with adjacent methoxy groups are capable of generating O- methyl carbamates and O-methyl thiocarbamates from the addition of those amines to CDI or TCDI followed by quenching with methanol during the solvent exchange In contrast to 1 and 2, amine-linked 3 is noncrystalline and 27,28 process. For this reason, the yields of cyclic carbamate less porous, with a BET area of only 61 m2/g. Based on these and cyclic thiocarbamate are reported as a range that considers results, it would appear the COF had irreversibly degraded the possibility that the O-methyl species may be contributing after the reduction; however, carrying the synthesis through to to the observed resonance. generate 4 or 5 yields materials which are both crystalline and Having determined the composition of these COFs, we porous. Pawley ﬁtting of the diﬀraction data for 4 and 5 shows sought to understand their structures in more detail and how good agreement with their respective model structures, they may have changed during the synthetic pathway. COFs conﬁrming that they possess both the connectivity and 1−5 were evaluated by powder X-ray diﬀraction (PXRD) and eclipsed stacking arrangement of their imine progenitor 1 N2 adsorption isotherm experiments (Figure 1b,c). Pawley (see SI, section S7). Additionally, the BET areas of 4 and 5 ﬁtting of imine-linked COFs 1 and 2 shows good agreement were found to be 780 and 791 m2/g, retaining 64 and 63% of with simulated structures, conﬁrming that their connectivity the BET area of 1, respectively. This retention of surface area and kgm topology are preserved during the demethylation step occurs despite the COF being subjected to three consecutive (see SI, section S7). Additionally, both 1 and 2 are porous, postsynthetic modiﬁcations, one of which resulted in a with Brunauer−Emmett−Teller (BET) areas of 1229 and 1233 noncrystalline framework. From these experiments, we can m2/g, respectively. While these experiments conﬁrm the infer that 3 possesses the same topology as 1, 2, 4, and 5, topology and porosity of these materials, they do not provide despite a lack of crystallinity. The loss of crystallinity and a complete picture of the structures of 1 and 2. Due to the porosity upon reduction of 2 and its subsequent reemergence broad diﬀraction peaks common to most COF materials, the in 4 and 5 can be attributed to the conformational ﬂexibility of diﬀraction data cannot provide enough information to the secondary amine linkages of 3. In contrast, imines, cyclic determine the orientation of the methoxy- or hydroxy- carbamates, and cyclic thiocarbamates are signiﬁcantly less substituted phenyl rings relative to the imine bond. The conformationally ﬂexible and adopt comparatively planar orientation of this ring relative to the linkage is critical to the conformations as observed in molecular model crystal formation of cyclic carbamates, as the cyclization cannot structures (see SI, section S11). proceed unless the amine and hydroxyl group are positioned This same pattern of crystallinity loss and recovery can be along the same side in close proximity. To gain insight into the observed from the reduction of the imine linkages of 1 to possible orientations of this site in each imine-linked COF amines, followed by reoxidation back to imines with 2,3- structure, molecular models of 1 and 2 were synthesized, and dichloro-5,6-dicyano-1,4-benzoquinone (DDQ).29 Both the their structures were determined by single-crystal X-ray starting and ending imine-linked materials are crystalline, diﬀraction (see SI, section S11). For the model of 1, it was while the intermediate amine is noncrystalline. Loss and found that the methoxy groups position themselves opposite recovery of crystallinity upon reduction and reoxidation of the the imine bond to minimize steric interactions, while the imine linkage is even observed for ILCOF-1, despite the hydroxy groups in 2’s model compound position themselves presence of strongly stacking pyrene units and a smaller pore on the same side as the imine to form intramolecular hydrogen size than 1 (see SI, section S13).30 Dynamics of this type have bonds. The diﬀerences in energy between the two possible previously been observed in molecular crystals, as well the phenyl orientations were explored for each model compound woven COF-505, for which crystallinity can be lost and by gas-phase DFT simulations (see SI, section S12). For the recovered by the removal and reintroduction of Cu+ templates hydroxy- and methoxy-substituted model compounds, the within the structure.31,32 orientations observed in the crystal structures were found to be In an eﬀort to evaluate the necessity of performing the preferred by 62.5 and 39.6 kJ/mol, respectively. 15N NMR demethylation of 1 in the solid state, we examined the chemical shifts for each orientation of the model compounds synthesis of 4 and 5 starting from de novo synthesized 2 (2′), were calculated (see SI, section S12) and suggest that these which can be formed directly from the condensation of TAPS species should be distinguishable by our 15N NMR experi- and 3,5-dihydroxyterephthalaldehyde (see SI, section S3). This ments. Comparing these predictions to experiment, not only would shift the demethylation, which we know to be are the methoxy-adjacent and hydroxy-adjacent imine sites incomplete in the solid state under our conditions, to the distinguishable between the 15N spectra of 1 and 2 but also 1 solution state. Even after extensive screening of crystallization contains two independent imine resonances. Based on the conditions, 2′ possesses poorer crystallinity and signiﬁcantly insights gained from the crystal structures and DFT lower surface area than 2 (see SI, section S10). The quality of calculations of the model compounds, we believe that both this COF has a signiﬁcant impact on subsequent postsynthetic orientations of the methoxy-substituted phenyl ring are present modiﬁcations (see SI, section S6). Despite being performed
11256 DOI: 10.1021/jacs.9b04731 J. Am. Chem. Soc. 2019, 141, 11253−11258 Journal of the American Chemical Society Article under identical conditions, reduction under this route proceeds Energy, Oﬃce of Science, Basic Energy Sciences under Award at only 80% yield. Subsequent treatment with CDI or TCDI DE-SC0001015. T.O.P. acknowledges funding from the NSF and DMAP yields 4′ and 5′, in which only 62 and 68% of 15N Graduate Research Fellowship Program and the Chevron-UC sites are carbamates and thiocarbamates, respectively. Berkeley Graduate Fellowship Program. We also acknowledge Furthermore, the BET areas of 4′ and 5′ are only 217 and use of the computational resources in the Molecular Graphics 332 m2/g respectively. The diﬀerences between these two and Computational Facility at UC Berkeley, which is synthetic routes illustrate the importance of the quality of COF supported under NIH S10OD023532. Crystal structures of starting material in postsynthetic modiﬁcations. In this case, model compounds 11 an 12 in the Supporting Information one additional synthetic step in the solid state provides access were obtained by Nicholas Settineri and were supported by the to signiﬁcantly higher yields and higher quality products due to NIH Shared Instrumentation Grant S10 RR027172. our ability to access a more crystalline and porous COF starting material. ■ REFERENCES (1) Yaghi, O. M.; Kalmutzki, M. J.; Diercks, C. S. Introduction to ■ CONCLUSIONS Reticular Chemistry: Metal-Organic Frameworks and Covalent Organic In conclusion, an imine-linked COF was transformed through Frameworks; Wiley-VCH Verlag GmbH & Co. KGaA: Weinheim, three consecutive synthetic steps to isostructural cyclic Germany, 2019; p 509. (2) Waller, P. J.; Gandara,́ F.; Yaghi, O. M. Chemistry of Covalent carbamate- and thiocarbamate-linked COFs. These new − linkages are the ﬁrst for which one-pot small-molecule Organic Frameworks. Acc. Chem. Res. 2015, 48, 3053 3063. (3) Diercks, C. S.; Yaghi, O. M. The atom, the molecule, and the equivalent reactions do not exist, necessitating the need for covalent organic framework. Science 2017, 355, 293−302. multistep synthesis in the solid state. Each substrate in this 15 (4) Lyle, S. J.; Waller, P. J.; Yaghi, O. M. Covalent Organic synthesis was analyzed by N multiCP-MAS NMR spectros- Frameworks: Organic Chemistry Extended into Two and Three copy, for the ﬁrst time allowing quantitative compositional Dimensions. Trends in Chemistry 2019, 1 (2), 172−184. analysis of each compound along the synthetic route. (5) Nagai, A.; Guo, Z.; Jin, S.; Feng, X.; Jin, S.; Chen, X.; Ding, X.; Furthermore, each solid-state chemical transformation per- Jiang, D. Pore surface engineering in covalent organic frameworks. formed in this work was accompanied by a structural or Nat. Commun. 2011, 2, 536. conformational transformation, highlighting the critical im- (6) Sun, Q.; Aguila, B.; Perman, J.; Earl, L. D.; Abney, C. W.; Cheng, portance of linkages in COF structure and properties. This Y.; Wei, H.; Nguyen, N.; Wojtas, L.; Ma, S. Postsynthetically work constitutes an extension of organic synthesisboth Modified Covalent Organic Frameworks for Efficient and Effective Mercury Removal. J. Am. Chem. Soc. 2017, 139 (7), 2786−2793. multistep transformations and the analytical rigor necessary to (7) Lohse, M. S.; Stassin, T.; Naudin, G.; Wuttke, S.; Ameloot, R.; characterize them from the solution to the solid state. De Vos, D.; Medina, D. D.; Bein, T. Sequential Pore Wall Modification in a Covalent Organic Framework for Application in ■ ASSOCIATED CONTENT Lactic Acid Adsorption. Chem. Mater. 2016, 28 (2), 626−631. *S Supporting Information (8) Waller, P. J.; Lyle, S. J.; Osborn Popp, T.; Diercks, C. S.; Reimer, The Supporting Information is available free of charge on the J. A.; Yaghi, O. M. Chemical Conversion of Linkages in Covalent − ACS Publications website at DOI: 10.1021/jacs.9b04731. Organic Frameworks. J. Am. Chem. Soc. 2016, 138, 15519 15522. (9) Haase, F.; Troschke, E.; Savasci, G.; Banerjee, T.; Duppel, V.; Synthetic procedures for monomers and model com- Dörfler, S.; Grundei, M. M. J.; Ochsenfeld, C.; Kaskel, S.; Lotsch, B. pounds, including NMR and mass spectra; synthetic V. Topochemical conversion of an imine- into a thiazole-linked procedures for all solid-state transformations, including covalent organic framework enabling real structure analysis. Nat. PXRD patterns; FT-IR spectra; N2 adsorption iso- Commun. 2018, 9, 2600. therms; and 15N-multiCP-MAS NMR spectra. Crystallo- (10) Liu, H.; Chu, J.; Yin, Z.; Cai, X.; Zhuang, L.; Deng, H. Covalent Organic Frameworks Linked by Amine Bonding for Concerted graphic information for each model compound and − associated computations (PDF) Electrochemical Reduction of CO2. Chem. 2018, 4, 1696 1709. (11) Li, X.; Zhang, C.; Cai, S.; Lei, X.; Altoe, V.; Hong, F.; Urban, J. J.; Ciston, J.; Chan, E. M.; Liu, Y. Facile transformation of imine ■ AUTHOR INFORMATION covalent organic frameworks into ultrastable crystalline porous Corresponding Author aromatic frameworks. Nat. Commun. 2018, 9, 2998. *[email protected] (12) Waller, P. J.; AlFaraj, Y. S.; Diercks, C. S.; Jarenwattananon, N. N.; Yaghi, O. M. Conversion of Imine to Oxazole and Thiazole ORCID Linkages in Covalent Organic Frameworks. J. Am. Chem. Soc. 2018, Steven J. Lyle: 0000-0003-2341-3177 140, 9099−9013. Peter J. Waller: 0000-0002-4013-8827 (13) Jaradat, D. M. M. Thirteen decades of peptide synthesis: key Jeﬀrey A. Reimer: 0000-0002-4191-3725 developments in solid phase peptide synthesis and amide bond formation utilized in peptide ligation. Amino Acids 2018, 50,39−68. 0000-0002-5611-3325 Omar M. Yaghi: (14) Fracaroli, A. M.; Siman, P.; Nagib, D. A.; Suzuki, M.; Furukawa, Notes H.; Toste, F. D.; Yaghi, O. M. Seven Post-synthetic Covalent The authors declare no competing ﬁnancial interest. Reactions in Tandem Leading to Enzyme-like Complexity within Metal-Organic Framework Crystals. J. Am. Chem. Soc. 2016, 138, ■ ACKNOWLEDGMENTS 8352−8355. Synthesis in this work was supported by King Abdulaziz City (15) Wei, P.-F.; Qi, M.-Z.; Wang, Z.-P.; Ding, S.-Y.; Yu, W.; Liu, Q.; Wang, L.-K.; Wang, H.-Z.; An, W.-K.; Wang, W. Benzoxazole-Linked for Science and Technology (Center of Excellence for Ultrastable Covalent Organic Frameworks for Photocatalysis. J. Am. Nanomaterials and Clean Energy Applications) and the Chem. Soc. 2018, 140, 4623−4631. characterization of compounds by the Center for Gas (16) Stewart, D.; Antypov, D.; Dyer, M. S.; Pitcher, M. J.; Separations Relevant to Clean Energy Technologies, an Energy Katsoulidis, A. P.; Chater, P. A.; Blanc, F.; Rosseinsky, M. J. Stable Frontier Research Center funded by the U.S. Department of and ordered amide frameworks synthesised under reversible
11257 DOI: 10.1021/jacs.9b04731 J. Am. Chem. Soc. 2019, 141, 11253−11258 Journal of the American Chemical Society Article conditions which facilitate error checking. Nat. Commun. 2017, 8, 1102. (17) Bala, M.; Verma, P. K.; Sharma, D.; Kumar, N.; Singh, B. Highly efficient water-mediated approach to access benzazoles: metal catalyst and base-free synthesis of 2-substituted benzimidazoles, benzoxazoles, and benzothiazoles. Mol. Diversity 2015, 19 (2), 263− 272. (18) Tang, J.; Wang, L.; Mao, D.; Wang, W.; Zhang, L.; Wu, S.; Xie, Y. Ytterbium pentafluorobenzoate as a novel fluorous Lewis acid catalyst in the synthesis of 2,4-disubstituted quinolines. Tetrahedron 2011, 67, 8465−8469. (19) Thakur, M. S.; Nayal, O. S.; Sharma, A.; Rana, R.; Kumar, N.; Maurya, S. K. An Efficient Metal-Free Mono N-Alkylation of Anilines via Reductive Amination Using Hydrosilanes. Eur. J. Org. Chem. 2018, 2018, 6729−6732. (20) Kandambeth, S.; Mallick, A.; Lukose, B.; Mane, M. V.; Heine, T.; Banerjee, R. Construction of Crystalline 2D Covalent Organic Frameworks with Remarkable Chemical (Acid/Base) Stability via a Combined Reversible and Irreversible Route. J. Am. Chem. Soc. 2012, 134, 19524−19527. (21) Baxter, E. W.; Rietz, A. B. Reductive aminations of carbonyl compounds with borohydride and borane reducing agents. Organic Reactions; John Wiley and Sons, Inc.: Hoboken, NJ, United States, 2002; pp 1−714. (22) Liu, Q.; Batt, D. G.; Delucca, G. V.; Shi, Q.; Tebben, A. J. Preparation of carbazole carboxamide compounds useful as kinase inhibitors. U. S. Patent 20100160303, June, 24, 2010. (23) Pretsch, E.; Bühlmann, P.; Badertscher, M. IR Spectroscopy. Structure Determination of Organic Compounds, 4th ed.; Springer: Berlin, 2009; pp 269−335. (24) Hu, X.-Y.; Zhang, W.-S.; Rominger, F.; Wacker, I.; Schröder, R. R.; Mastalerz, M. Transforming a chemically labile [2 + 3] imine cage into a robust carbamate cage. Chem. Commun. 2017, 53, 8616−8619. (25) Johnson, R. L.; Schmidt-Rohr, K. Quantitative solid-state 13C NMR with signal enhancement by multiple cross polarization. J. Magn. Reson. 2014, 239,44−49. (26) Duan, P.; Schmidt-Rohr, K. Composite-pulse and partially dipolar dephased multiCP for improved quantitative solid-state 13C NMR. J. Magn. Reson. 2017, 285,68−78. (27) Szabo, M.; Agostino, M.; Malone, D. T.; Yuriev, E.; Capuano, B. The design, synthesis and biological evaluation of novel URB602 analogues as potential monoacylglycerol lipase inhibitors. Bioorg. Med. Chem. Lett. 2011, 21, 6782−6787. (28) Hernandez,A.S.;Hodges,J.C.Solid-Supportedtert-́ Alkoxycarbonylation Reagents for Anchoring of Amines during Solid Phase Organic Synthesis. J. Org. Chem. 1997, 62, 3153−3157. (29) Luca, O. R.; Wang, T.; Konezny, S. J.; Batista, V. S.; Crabtree, R. H. DDQ as an electrocatalyst for amine dehydrogenation, a model system for virtual hydrogen storage. New J. Chem. 2011, 35, 998−999. (30) Rabbani, M. G.; Sekizkardes, A. K.; Kahveci, Z.; Reich, T. E.; Ding, R.; El-Kaderi, H. M. A 2D Mesoporous Imine-Linked Covalent Organic Framework for High Pressure Gas Storage Applications. Chem. - Eur. J. 2013, 19, 3324−3328. (31) Alam, P.; Leung, N. L. C.; Cheng, Y.; Zhang, H.; Liu, J.; Wu, W.; Kwok, R. T. K.; Lam, J. W. Y.; Sung, H. H. Y.; Williams, I. D.; Tang, B. Z. Spontaneous and Fast Molecular Motion at Room Temperature in the Solid State. Angew. Chem., Int. Ed. 2019, 58, 4536. (32) Liu, Y.; Ma, Y.; Zhao, Y.; Sun, X.; Gandara, F.; Furukawa, H.; Liu, Z.; Zhu, H.; Zhu, C.; Suenaga, K.; Oleynikov, P.; Alshammari, A. S.; Zhang, X.; Terasaki, O.; Yaghi, O. M. Weaving of Organic Threads into a Crystalline Covalent Organic Framework. Science 2016, 351, 365−369.
11258 DOI: 10.1021/jacs.9b04731 J. Am. Chem. Soc. 2019, 141, 11253−11258